A problem arises for crystals having hexagonal symmetry in that some crystallo-
graphic equivalent directions will not have the same set of indices. This is circum-
*vented by utilizing a four-axis, or Miller–Bravais, coordinate system as shown in*

*Figure 3.21. The three a*1*, a*2*, and a*3axes are all contained within a single plane
*z*
*+ y*
* y* *O*
*a*
* a*
*a*
[110] Direction
*P*
*x*
*a*
*a*
*a*_{1}
*a*_{2}
*a*_{3}
*z*
120°

**FIGURE3.21** Coordinate axis system for a hexagonal unit cell

(called the basal plane), and at 120⬚*angles to one another. The z axis is perpendicular*
to this basal plane. Directional indices, which are obtained as described above, will
*be denoted by four indices, as [uvtw]; by convention, the first three indices pertain*

*to projections along the respective a*1*, a*2*, and a*3axes in the basal plane.

Conversion from the three-index system to the four-index system,
*[u*⬘*v*⬘*w*⬘] —씮*[uvtw]*

is accomplished by the following formulas:

*u*⫽*n*
3*(2u*⬘ ⫺*v*⬘) (3.7a)
*v*⫽*n*
3(2*v*⬘ ⫺*u*⬘) (3.7b)
*t*⫽ ⫺*(u*⫹*v*) (3.7c)
*w*⫽*nw*⬘ (3.7d)

where primed indices are associated with the three-index scheme and unprimed,
*with the new Miller–Bravais four-index system; n is a factor that may be required*
*to reduce u,v, t, and w to the smallest integers. For example, using this conversion,*
the [010] direction becomes [1210]. Several different directions are indicated in the
*hexagonal unit cell (Figure 3.22a).*

**3.13 C**

**RYSTALLOGRAPHIC**

**P**

**LANES**

The orientations of planes for a crystal structure are represented in a similar manner.
Again, the unit cell is the basis, with the three-axis coordinate system as represented
in Figure 3.19. In all but the hexagonal crystal system, crystallographic planes are
* specified by three Miller indices as (hkl). Any two planes parallel to each other*
are equivalent and have identical indices. The procedure employed in determination

*of the h, k, and l index numbers is as follows:*

**1. If the plane passes through the selected origin, either another parallel**

plane must be constructed within the unit cell by an appropriate transla- tion, or a new origin must be established at the corner of another unit cell.

**2. At this point the crystallographic plane either intersects or parallels each**

of the three axes; the length of the planar intercept for each axis is
*determined in terms of the lattice parameters a, b, and c.*

**54** ● **Chapter 3 / Structures of Metals and Ceramics**

[0001]
(0001)
[1120]`
[1100]`
(1010)
(1011)`
*a*_{1}
*a*_{1}
*a*_{2}
*a*_{3}
*a*_{3}
*z*
*z*
*(a)* *(b)*
`

**FIGURE3.22** For the

hexagonal crystal system,
*(a) [0001], [1100], and [1120]*
*directions, and (b) the (0001),*
(1011), and (1010) planes.

**3.13 Crystallographic Planes** ● **55**
*z*
*x*
*y*
*z*
*x*
*y*
*z*
*x*
*y*
*(b)*
*(c)*
*(a)*
*O*
(001) Plane referenced to
the origin at point *O*

(111) Plane referenced to
the origin at point *O*

(110) Plane referenced to the
origin at point *O*
Other equivalent
(001) planes
Other equivalent
(111) planes
Other equivalent
(110) planes
*O*
*O*
**FIGURE3.23** Representations of a
*series each of (a) (001), (b) (110),*
*and (c) (111) crystallographic planes.*

**3. The reciprocals of these numbers are taken. A plane that parallels an**

axis may be considered to have an infinite intercept, and, therefore, a zero index.

**4. If necessary, these three numbers are changed to the set of smallest**

integers by multiplication or division by a common factor.2

**5. Finally, the integer indices, not separated by commas, are enclosed within**

*parentheses, thus: (hkl).*

An intercept on the negative side of the origin is indicated by a bar or minus sign positioned over the appropriate index. Furthermore, reversing the directions of all indices specifies another plane parallel to, on the opposite side of and equidis- tant from, the origin. Several low-index planes are represented in Figure 3.23.

One interesting and unique characteristic of cubic crystals is that planes and directions having the same indices are perpendicular to one another; however, for other crystal systems there are no simple geometrical relationships between planes and directions having the same indices.

2_{On occasion, index reduction is not carried out}_{兵}_{(e.g., for x-ray diffraction studies that are}

described in Section 3.19);其for example, (002) is not reduced to (001). In addition, for ceramic materials, the ionic arrangement for a reduced-index plane may be different from that for a nonreduced one.

**56** ● **Chapter 3 / Structures of Metals and Ceramics**
*z*
*y*
*x*
*a*
*b*
*O*
*c*
*z*
*y*
*x*
*(a)* *(b)*
*x*
*b*
*c*/2
(012) Plane
*z*
*O*
*O*
⬘
⬘
⬘

**E**

**XAMPLE**

**P**

**ROBLEM**

**3.9**

Determine the Miller indices for the plane shown in the accompanying
*sketch (a).*

**S**

**O L U T I O N**

*Since the plane passes through the selected origin O, a new origin must be*
*chosen at the corner of an adjacent unit cell, taken as O*⬘and shown in sketch
*(b). This plane is parallel to the x axis, and the intercept may be taken as*앝*a.*

*The y and z axes intersections, referenced to the new origin O*⬘, are ⫺*b and*
*c/2, respectively. Thus, in terms of the lattice parameters a, b, and c, these*

intersections are앝,⫺1, and. The reciprocals of these numbers are 0,⫺1, and 2; and since all are integers, no further reduction is necessary. Finally, enclosure in parentheses yields (012).

These steps are briefly summarized below:

*x* *y* *z*

Intercepts 앝*a* ⫺*b* *c/2*

Intercepts (in terms of lattice parameters) 앝 ⫺1 Reciprocals 0 ⫺1 2 Reductions (unnecessary)

Enclosure (012)

**E**

**XAMPLE**

**P**

**ROBLEM**

**3.10**

Construct a (011) plane within a cubic unit cell.

**S**

**O L U T I O N**

To solve this problem, carry out the procedure used in the preceding example
in reverse order. To begin, the indices are removed from the parentheses, and
reciprocals are taken, which yields앝,⫺1, and 1. This means that the particular
*plane parallels the x axis while intersecting the y and z axes at* ⫺*b and c,*

*respectively, as indicated in the accompanying sketch (a). This plane has been*
*drawn in sketch (b). A plane is indicated by lines representing its intersections*
with the planes that constitute the faces of the unit cell or their extensions. For
*example, in this figure, line ef is the intersection between the (011) plane and*

**3.13 Crystallographic Planes** ● **57**

*the top face of the unit cell; also, line gh represents the intersection between*
this same (011) plane and the plane of the bottom unit cell face extended.
*Similarly, lines eg and fh are the intersections between (011) and back and*
front cell faces, respectively.